www.euacademic.org DRJI Value: 5.9 (B+)
Study of influence of refluxing on uncapped CdTe
nanoparticles synthesized by a facile route
MUHAMMAD ZAIN AKRAM1
Centre of Excellence in Solid State Physics University of the Punjab, Lahore, Pakistan MALEEHA QASIM Laboratory of Micro and Nano Electro Mechanical Systems Northwestern Polytechnical University, Xi’an, China MUHAMMAD AHSAN IQBAL HAREEM ARIF SAHER HAMID Centre of Excellence in Solid State Physics University of the Punjab, Lahore, Pakistan MUHAMMAD AMIN South China Sea Institute of Oceanology Chinese Academy of Sciences, Guangzhou, Guangdong, P. R China ROSHAN ALI School of Electronics, Electrical and Communication Engineering University of Chinese Academy of Sciences, Beijing, China MUHAMMAD IRFAN2
Department of Physics, B.Z.U Multan, Pakistan
Semiconductor CdTe is of great interest for use in optoelectronic devices. CdTe nanoparticles ~10 – 25 nm differ remarkably in properties from their bulk making them potential candidates for photovoltaic applications. CdTe nanoparticles are synthesized by low cost, simple and application oriented co-precipitation technique. De-ionized water was used as solvent whereas cadmium chloride (CdCl2) was used as cadmium source. CdTe sol was prepared by refluxing the product at C for 0 – 120 minutes.
Solution was then centrifuged at 5000 rpm for 10 minutes. Resultant precipitates were annealed at 50 - 100oC for different time intervals. CdTe nanocrystals with hexagonal phase were confirmed by X-Ray Diffractograms. Grain size was tuned to ~11 nm, as observed by SEM, by changing the synthesis conditions and refluxing time. Previous studies showed preparation of CdTe nanoparticles in the presence of organic solvents and some surfactants, whereas in this research work simplest route of CdTe nanoparticles’ synthesis only by using de-ionized water is explained. Optical properties revealed that the band-gap of these CdTe nano-particles is slightly different from the bulk values. High absorption of the solar spectrum warrants their use in solar cells with the added advantage of increased surface area.
Key words: CdTe nano-particles, Refluxing, surfactant free, solution chemistry
Optical and electronic properties of semiconducting nanoparticles are strongly size dependent because of the quantum confinement effect. Highly luminescent II-VI semiconductor nanoparticles have been extensively studied since they are promising materials for next generation optical and electronic devices (Gaponik 2011, Gallardo 2007). Most of the research involves cadmium telluride nanocrystals since the high photoluminescence (PL) quantum efficiencies of CdTe make it an interesting material for use in applications such as light emitting devices (Chen 2002, Gaponik 1999, Gaponik 2000, Rogach 2007) photovoltaic devices (Khan 2011, Kumar 2004) and biological labels (Wang 2006, Green 2007).
of nanoparticles via physical methods such as ball milling (Tan 2003) and laser ablation (Ruth 2006).
Organometallic routes are generally toxic and expensive providing less stability in air and less reproducibility. Whereas, reactions comprising of aqueous chemistry are not only environmentally benign but they also have merits like stability, simplicity and reproducibility. When the nanoparticles prepared via aqueous solution chemistry are extracted as free-standing powders, they can be exploited in thin film preparation for device formation application. Most of the aqueous syntheses are carried out using capping agents like TOPO or thiol stabilizers such as Mercaptopropionic acid (MPA), Mercaptoacetic Acid (MMA) or 2-Mercaptoethanol (ME) (Abd El-sadek 2011). The use of these capping agents is to control the shape and size of growing particles through charge transfer and to prevent agglomeration of particles thus making them stable and passivating them against oxidation. Capping agents, however, are not always sought-after since for many applications efficiency of nanoparticles is affected by the surfactant molecules that are covalently bonded with the surface atoms of nanoparticles. For example, for organic photovoltaic hybrid solar applications, where charge transfer between nanoparticles and conjugated polymer are required, surfactant may cause hindrance in the charge transfer. Therefore, often the exchange or removal of surfactant from the surface of nanoparticles is an additional step.
Keeping in view the potential of nanocrystals to be used in solar cell applications, efforts are made to produce surfactant free nanocrystals and the size of particles is controlled with the help of refluxing. 0.5M CdCl2. 2.5 H20 is used as cadmium source and potassium tellurite is used as tellurium source to prepare nanocrystals of different sizes at different pH values. Size is controlled via refluxing and reaction conditions. As prepared CdTe nanocrystals are isolated by the addition of methanol followed by centrifugation and drying in vacuum at room temperature.
Cadmium chloride, potassium tellurite, potassium hydroxide, deionised (DI) water, nitrogen gas, methanol were all used as-purchased without any further purification.
2.2. Synthesis of CdTe nanoparticles
0.5M CdCl2 . 2.5 H20 solution was prepared in 20mL DI water at room temperature. pH of the solution was maintained at ~10 by drop wise addition of 1M KOH solution. The solution was then placed in a three-necked flask and was bubbled with N2. 0.4 M potassium tellurite solution was prepared in 20 mL DI water and was stirred for 2 hours. Dark grey color of the solution indicated the nucleation of CdTe after refluxing and condensation. Resulting powder was separated by centrifugation at 5000 rpm for 10 minutes and dried in vacuum at room temperature. 5 samples naming S1, S2, S3, S4, and S5 with different refluxing time were obtained.
Voltage of 35kV and 25 mA current was used to produce X-rays. Size and morphology of nanoparticles was observed by Hitachi S-3400N Scanning electron microscope (SEM). Optical characterization was done by using JA Woolam’s variable angle spectroscopic ellipsometer (VASE).
3.Results And Discussion
3.1. Structural properties
XRD pattern of as-synthesized CdTe nanoparticles, at different reflux times, is shown in Fig.1. XRD patterns shows two distinct peaks at angles (2 ) of and , which can be indexed to diffraction from (1 1 0) and (1 1 2) planes of hexagonal crystal lattice, respectively. This matches quite well with the international centre for diffraction data (JCPDS card card no. 19-193).
Fig. 1 X-ray diffraction patterns of CdTe nanoparticles refluxed at (a) 15 min (b) 30 min (c) 45 min (d) 60 min (e) 120 min
+ hk +
) + /
From the XRD pattern it can be concluded that as the reflux time increases the crytsallinity of the particles increases, and the sample refluxed for 2 hours shows a sharp peak at (1 1 0) plane which confirms the hexagonal structure of CdTe nanoparticles. Crystallite size is found to be in range of 11 – 19nm, calculated by Scherer equation stated below:
D = K
Where K is a constant that is equal to 0.94, lambda is the X-ray wavelength 𝛌 = 1.5405Å and B is the full width at half maximum (FWHM) of the XRD selected diffraction peak on the 2 scale, is the diffraction angle.
Fig. 1 (a) FWHM and (b) crystallite size of CdTe nanoparticles at different reflux times
The dissimilarity in growth of crystallites can be referred to the stresses and relaxations produced in the films. The stress/strain ratio varies notably as a function of crystallite growth since the films provide accommodation to the high temperature stresses in the grains. Crystallite growth is driven by neighboring crystals that possess different energies due to the curvature of energetic grain boundaries and different amounts of accumulated strain energy. By differentiating the Bragg’s law the micro strains are calculated as:
The uniform strain is observed in the films and this fact is evident from the shapes and shifts of the peaks of reflection planes when compared with the standard shapes. (Cullity 1978).
3.2. Surface properties
increasing the reflux time to 45 min an increase in particle diameter was observed, with an average value of ~25 nm. Size of nanoparticles kept growing with the increase in reflux time for 60 (~50nm) and 120 min (~100nm). The increase in particle size for samples (S3-S5) with increased refluxing time is found to be in correlation with the results reported earlier, where the EMA sizes of the particles were found to increase with the increased in reflux duration (Abd El-sadek 2011). This suggests that nanoparticles’ size keeps on growing with the increase in reaction time. Such growth of particles suggests that mechanism of growth is “Ostwald ripening”, where a large number of colloidal particles fight for a finite number of monomers. The high surface energy of smaller particles promotes their dissolution and larger particles will continue to grow as more and more material adds to the existing nuclei and slowly there is a reduction in total number of particles.
Fig. 3 SEM micrographs of CdTe nanoparticles refluxed for (a) 15 min, (b) 30 min, (c) 45 min, (d) 60 min (e) 120 min and (f) Plot between nanoparticles’ diameter and reflux time.
Fig. 4(f) shows a plot of nanoparticle diameter against reflux time. A sharp decrease in particle size was observed when the reflux time was changed from 15 min to 30 min and after that a steady increase in particle size was observed. The trend is similar to that of “crystallite size versus reflux time”, calculated from XRD pattern.
3.3. Optical Properties
Absorption spectra of CdTe nanoparticles are plotted in Fig. 4. Pure CdTe has a high absorption coefficient in the visible and near infrared region; the same was observed in this research work [Fig. 4]. It can be seen through the absorption plot that by
increasing the reflux time absorption of CdTe nanoparticles also increases. However, band edge energies are not shifting linearly. The band edge shifts towards high energy side, i.e. blue shift, for CdTe nanoparticles prepared at 15, 30 and 120 minutes reflux time. Relatively larger band shift was observed for 30 minutes reflux time which might have had happened because of the quantum confinement effect on the electronic band structure (Rastogi 2000) for CdTe nanopaticles’ diameter ~ 11 nm [Fig. 3b].
Fig. 4 Absorption spectra of CdTe nanoparticles refluxed for different time
Fig. 5 Variation in band gap energies of CdTe nanoparticles refluxed for different time
Band gap of CdTe (1.42 eV) makes it the most suitable material for photovoltaic conversion (Rastogi 2000). However, the absolute value of band gap energy would slightly depend upon the deposition process and conditions in case of a thin film.
It can be seen from Fig. 5 that band gap energy in the range of 1.41 – 1.51eV is observed for these CdTe nanoparticles prepared under 30 and 60 refluxed times. Band gap energies, with respect to particle size and shape, is given in Table - I. The sharp increase in band gap energies indicates the direct band gap of chemically synthesized CdTe nanoparticles.
Table - I Effect of reflux time on CdTe nanoparticles’ size, shape and band gap energy
We have successfully synthesized CdTe nanoparticles, without using any capping agent, via simple and environmental friendly route. Particle size was monitored with respect to refluxing time, and their size ranging from ~11nm to ~50nm was observed after refluxing for 15 to 60 minutes. All particles were found to be spherical in shape. XRD patterns confirmed the formation of hexagonal cadmium telluride for all the refluxed times. High absorption values along with a direct band gap of 1.42 eV was observed for the nanoparticles prepared at 30 and
Sample Reflux Time (minutes)
Nanoparticles’ Diameter (nm)
Band Gap (eV)
S1 15 50 Spherical 1.41
S2 30 11 Spherical 1.42
S3 45 25 Spherical 1.47
S4 60 50 Spherical 1.42
60 refluxed time. Whereas, a small increase in band gap energies was found for reflux time 45 min (1.47eV) and 120min (1.51eV).
Abd El-sadek, M.S., Nooralden, A.Y., Babu, S.M. and Palanisamy, P.K. (2011), ”Influence of different stabilizers on the optical and nonlinear optical properties of CdTe nanoparticles.” J. Opt. Com., Vol.
Bertoni, C., Gallardo, D., Dunn, S., Gaponik, N.P., and Eychmüllr, A. (2007) “Fabrication and characterization of red-emitting electroluminescent devices based on thiol-stabilized semiconductor nanocrystals” J. Appl. Phys. Lett., Vol. 90(3), 034107 - 034107-3
Chen, W., Grouquist, D. and Roark, J. (2002) “Voltage tunable electroluminescence of CdTe nanoparticle light-emitting diodes”. JNN., Vol. 2(1), 47-53.
Cullity. B.D. (1978), “Elements of X-ray diffraction”, Addison Wesley Publishing Co., USA.
Green, M., Harwood, H., Barrowman, C., Rahman, P., Eggeman, A., Festry, F., Dobson P., and Ng T. (2007) “A facile route to CdTe nanoparticles and their use in bio-labelling”. J. Mater. Chem., Vol.17, 1989-1994.
Gaponik, N.P., Herrmann, A.K. and Eychmüller, A. (2011) “Colloidal nanocrystal-based gels and aerogels: material aspects and application perspectives.” J. Phys. Chem. Lett., Vol. 3, 8−17.
Gaponik, N.P., Talapin, D.V., Rogach, A.L. and Eychmüller, A. (2000) “Electrochemical synthesis of CdTe nanocrystal/polypyrrole composites for optoelectronic applications”. J. Mater. Chem., Vol. 10, 2163-2166. Khan, M.T., Kaur, A., Dhawan, S.K. and Chand, S. (2011)
“In-Situ growth of cadmium telluride nanocrystals in poly(3-hexylthiophene) matrix for photovoltaic application” J. Appl. Phys., Vol. 110, 044509-1-6.
Kumar, S. and Nann, T. (2004), “First solar cells based on CdTe nanoparticle/MEH-PPV composites”. J. Mater. Res., Vol.
Mathew, X., Enriquez J.P., Romeo, A. and Tiwari, A.N. (2004), “CdTe/CdS solar cells on flexible substrates”. J. Sol. Energ., Vol. 77, 831–838.
Mntungwa, N., Rajasekhar, P. and Revaprasadu, N. (2011), “A facile route to shape controlled CdTe nanoparticles”. J. Mat. Chem. Phys., Vol. 126, 500–506.
Rastogi, A.C., Sharma, S.N. and Kholi, S. (2000), “Size dependent optical edge shifts and electrical conduction behavior of RF magnetron sputtered CdTe nanocrystals: TiO2 composite thin films”. Vol. 15, 1011–1021.
Rogach, A.L. (2000), “Nanocrystalline CdTe and CdTe(S) particles: wet chemical preparation, size-dependent optical properties and perspectives of optoelectronic applications.” Materials Science and Engineering, Vol.
Rogach, A.L., Gaponik, N., Lupton, J.M., Bertoni, C., Gallardo, D.E., Dunn, S., Pira, N., Li., P.M., Repetto, P., Romanov, S.G., O’Dwyer, C., Sotomayor T., Clivia, M. and Eychm A. (2008), “Light-emitting diodes with semiconductor nanocrystals.” J. Angew. Chem. Int., Vol. 47, 6538 – 6549.
Colloids and Surfaces A: Physicochem. Eng. Aspects Vol.
Sathyamoorthy, R., Sudhagar, P., Kumar, R.S., and Sathyadevan T.M. (2010), “Low temperature synthesis of thiol-functionalized CdTe nanoclusters with different tellurium contents”, Cryst. Res. Technol. Vol. 45(1), 99 – 103.
Talapin, D.V., Haubold, S., Rogach, A.L., Kornowski, A., Haase, M. and Weller, H. (2001), “A novel organometallic synthesis of highly luminescent CdTe nanocrystals” J. Phys. Chem. B Vol. 105, 2260-2263.
Tan, G.L., Hommerich, U., Temple, D., Wu, N.Q., Zheng J.G. and Loutts G. (2003), “Synthesis and optical characterization of CdTe nanocrystals prepared by ball milling process.” Scripta Materialia Vol. 48 1469–1474. Verma, D., Rao, A.R. and Dutta, V. (2009) ,” Surfactant-free
CdTe nanoparticles mixed MEH-PPV hybrid solar cell deposited by spin coating technique” J. Sol. Mat., Vol.
Wang, X., Ma, Q., Li, B., Li, Y., and Su, X. (2006) “The preparation of CdTe nanoparticles and CdTe nanoparticle-labelled microspheres for biological applications”. Luminescence Vol. 22, 1–8.